A ruthenium(IV) complex with six sulfur donor atoms
Maiti, Rabindranath; Shang, Maoyu; Graham Lappin, A.; Chemical Communications  (1999) 2349–; doi:10.1039/a905243g

data_7110644
_publ_section_title
;
 A ruthenium(IV) complex with six sulfur donor atoms
;
_journal_issue                   23
_journal_name_full               'Chemical Communications'
_journal_page_first              2349
_journal_paper_doi               10.1039/a905243g
_journal_year                    1999
_chemical_formula_sum            'C32 H41 N10 O0.5 Ru S6'
_chemical_formula_weight         867.18
_chemical_name_systematic
;

(Et4N)2[Ru(mnd)2].0.5H2O

;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 111.319(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.1816(15)
_cell_length_b                   27.145(5)
_cell_length_c                   12.767(3)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      14
_cell_measurement_theta_min      12
_cell_volume                     4255.6(14)
_computing_cell_refinement       'CAD4-ARGUS (Enraf-Nonius, 1994)'
_computing_data_collection       'CAD4-ARGUS (Enraf-Nonius, 1994)'
_computing_data_reduction
;

Chi90s (Boyle, 1996), Xcad4 (Harms, 1996), SHELXTL_V5 (Siemens, 1994)

;
_computing_molecular_graphics
;

ORTEP-III (Farrugia, Burnett, Johnson, 1996)

;
_computing_publication_material  'SHELXTL_V5 (Siemens, 1994)'
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device       'Enraf-Nonius CAD4'
_diffrn_measurement_method       \w/2\q
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0585
_diffrn_reflns_av_sigmaI/netI    0.0626
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            7790
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.04
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 200
_diffrn_standards_interval_time  120
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    0.699
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.4206
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    1.353
_exptl_crystal_density_meas      ?
_exptl_crystal_description       plate-like
_exptl_crystal_F_000             1788
_exptl_crystal_size_max          0.45
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.854
_refine_diff_density_min         -0.679
_refine_diff_density_rms         0.101
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.065
_refine_ls_goodness_of_fit_obs   1.195
_refine_ls_hydrogen_treatment
;

Ethyl hydrogen atoms were refined with idealized riding models and those

of water were refines isotropically with bond length restraints.

;
_refine_ls_matrix_type           full
_refine_ls_number_parameters     506
_refine_ls_number_reflns         7444
_refine_ls_number_restraints     372
_refine_ls_restrained_S_all      1.076
_refine_ls_restrained_S_obs      1.178
_refine_ls_R_factor_all          0.1077
_refine_ls_R_factor_obs          0.0705
_refine_ls_shift/esd_max         -0.005
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1167P)^2^+3.2582P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.2184
_refine_ls_wR_factor_obs         0.1907
_reflns_number_observed          4794
_reflns_number_total             7448
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            905243gsup1.cif
_cod_data_source_block           la9804
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.1167P)^2^+3.2582P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.1167P)^2^+3.2582P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_original_formula_sum        'C32 H41 N10 O0.50 Ru S6'
_cod_database_code               7110644